# Control of Thermophysical Properties of Langasite-Type La3Ta0.5Ga5.5O14 Crystals for Pressure Sensors

Haruki Usui, Makoto Tokuda, Kazumasa Sugiyama, Takuya Hoshina, Takaaki Tsurumi, Kheirreddine Lebbou, Ikuo Yanase, Hiroaki Takeda

► To cite this version:

Haruki Usui, Makoto Tokuda, Kazumasa Sugiyama, Takuya Hoshina, Takaaki Tsurumi, et al., Control of Thermophysical Properties of Langasite-Type La3Ta0.5Ga5.5O14 Crystals for Pressure Sensors. Crystals, 2020, 10 (10), pp.936. 10.3390/cryst10100936. hal-03011177

HAL Id: hal-03011177

https://hal.science/hal-03011177

Submitted on 18 Nov 2020

HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

L'archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d'enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

<figure><img src="image_1.png" /></figure>

Distributed under a Creative Commons Attribution 4.0 International License
Article

# Control of Thermophysical Properties of Langasite-Type La₃Ta₀.₅Ga₅.₅O₁₄ Crystals for Pressure Sensors

Haruki Usui <fnref n="1" />, Makoto Tokuda <fnref n="2" />, Kazumasa Sugiyama <fnref n="2" />, Takuya Hoshina ¹ID, Takaaki Tsurumi <fnref n="1" />, Kheirreddine Lebbou <fnref n="3" />, Ikuo Yanase <fnref n="4" /> and Hiroaki Takeda <fnref n="1" />,4,*

Received: 25 August 2020; Accepted: 13 October 2020; Published: 14 October 2020

<figure><img src="image_2.png" /></figure>

check for
updates

**Abstract:** We present a possible method to reduce the anisotropy of the thermal stress generated on langasite-type La₃Ta₀.₅Ga₅.₅O₁₄ (LTG) piezoelectric crystals arising from the mismatch of the thermal expansion coefficients and Young's moduli of the crystals and metals at high temperatures. To formulate this method, the thermal stresses of order-type langasite crystals, in which each cation site is occupied by one element only, were calculated and compared to each other. Our results suggest that the largest cation site affects the thermal stress. We attempted to replace La<fnref n="3" />⁺ in LTG by a larger ion and considered Sr<fnref n="2" />⁺. Single crystals of strontium-substituted LTG (Sr-LTG) were grown using the Czochralski method. The thermal stress along the crystallographic c-axis decreased but that perpendicular to the c-axis increased by strontium substitution into the LTG crystal. The anisotropic thermal stress was reduced effectively. The Sr-LTG single crystal is a superior candidate material for pressure sensors usable at high temperatures.

**Keywords:** anisotropy; thermal stress; langasite; pressure sensor; substitution

## 1. Introduction

In recent years, the automobile industry has been faced with a number of environmental and energy problems. Consequently, improvements to fuel efficiency and reduction in exhaust gas have been required [1]. Combustion pressure sensors are attractive devices for improving the combustion efficiency of engines. Such devices are directly placed in engine cylinders and combustion efficiency is improved by feedback control of the fuel injection based on data of the combustion pressure changes in the cylinder. An engine with a combustion pressure sensor can reduce NOx emissions by approximately 30%, and the emission of CO₂, which is a cause of global warming, by about 10% [2].

La₃Ga₅SiO₁₄ (langasite) family single crystals are attractive piezoelectric materials for use in combustion pressure sensors because they show no phase transitions up to their melting temperature and can be easily grown to large sizes using the Czochralski (Cz) technique [3–9]. GaPO₄ crystals [10] and rare-earth (Re) calcium oxoborate ReCa₄O(BO₃)₃ crystals [11] have also been reported to be promising candidates because the former has a high phase transition temperature of 930 °C and the latter maintains the piezoelectric property to its melting temperature of approximately 1600 °C.

<footnote n="1">¹ School of Materials and Chemical Technology, Tokyo Institute of Technology, Meguro, Tokyo 152-8552, Japan; usui.h.ab@m.titech.ac.jp (H.U.); thoshina@ceram.titech.ac.jp (T.H.); ttsurumi@ceram.titech.ac.jp (T.T.)</footnote>

<footnote n="2">² Institute for Materials Research (IMR), Tohoku University, Sendai 980-8577, Japan; tokuda@imr.tohoku.ac.jp (M.T.); kazumasa@imr.tohoku.ac.jp (K.S.)</footnote>

<footnote n="3">³ Institut Lumière Matière, UMR5306 CNRS, Université de Lyon 1, 69622 Villeurbanne CEDEX, France; kheirreddine.lebbou@univ-lyon1.fr</footnote>

<footnote n="4">⁴ Graduate School of Science and Engineering, Saitama University, 255 Shimo-Okubo, Sakura-ku, Saitama 338-8570, Japan; yanase@apc.saitama-u.ac.jp</footnote>

<footnote>* Correspondence: takeda@apc.saitama-u.ac.jp; Tel.: +81-48-858-3501</footnote>
However, bulk growth of $GaPO_4$ crystals is very difficult [12], while $ReCa_4O(BO_3)_3$ crystals have very low crystal symmetries (monoclinic $m$), and then show pyroelectricity [13]. Recently, gehlenite $Ca_2Al_2SiO_7$ and related crystals in the melilite group have been the subject of much study, because they exhibit piezoelectricity without any accompanying pyroelectricity [14,15]. The crystals also have very clear cleavage planes, which is a matter of concern for target applications in combustion pressure sensors.

Among the langasite family crystals, the $La_3Ta_{0.5}Ga_{5.5}O_{14}$ (LTG) single crystal is the most promising candidate [16,17] because it shows weak temperature dependence of its piezoelectric properties, and high electrical resistivity at high temperatures. Fracture of the crystal element during use is a matter of concern for combustion pressure sensors [18]. The fractures can be attributed to the high impulsive force generated during abnormal combustion. During use, thermal stresses along and perpendicular to the crystallographic $c$-axis are anisotropically generated at a working temperature of approximately 200 °C. At high temperatures, anisotropic thermal stress is caused by the difference in the thermal expansion coefficients and Young’s moduli among the LTG crystals used as the substrate and the metals used as crystal support. Reducing the anisotropic thermal stress by applying element substitution into the LTG may be an effective way to avoid this phenomenon.

In this study, first, we describe the calculation of the thermal stress using the data of the linear thermal expansion coefficients and elastic stiffness coefficients instead of the Young’s moduli, of four order-type langasite family crystals and the metal at high temperatures. Then, the candidate of the substituent element Sr was selected. We have also reported the effect of Sr substitution on the LTG crystals, which demonstrated a successful reduction in the anisotropic thermal stress.

## 2. Materials and Methods

### 2.1. Thermal Stress Calculation

A simplified structure surrounding the piezoelectric crystal substrate of the combustion pressure sensor was constructed for thermal stress calculation [19], as shown in Figure 1a. The piezoelectric X-cut of the crystal substrate and metal were in contact. The X-cut corresponds to the Miller plane $(1\bar{2}0)$ perpendicular to the crystallographic $a$-axis. The $a$- and $c$-axes correspond to the $x$- and $z$-axes, respectively. Langasite family crystals belong to a trigonal crystal system. Hence, the $y$-axis is the [120] direction. As the piezoelectric coefficient used in the combustion pressure sensor is $d_{11}$, the $x$-, $y$-, and $z$-axes are as indicated in Figure 1. At the initial state, the length of the crystal is the same as that of the metal. As the crystal is strongly fixed by the metal part, the crystal attempts to extend with the metal during temperature rise. Under the conditions shown in Figure 1b, the expansions of the crystal $\Delta l_c$ and the metal $\Delta l_m$ caused by their own thermal expansions are expressed using the following Equations (1) and (2):

$$ \Delta l_c = \alpha_c \Delta Tl_0, \qquad (1) $$

$$ \Delta l_m = \alpha_m \Delta Tl_0, \qquad (2) $$

where $\alpha_c$ and $\alpha_m$ are the linear thermal expansion coefficients (LTEC) of crystal and metal, respectively. $\Delta T$ is the change in temperature and $l_0$ is the length of both the crystal and metal at the initial temperature. As the metal is composed of polycrystals, $\alpha_m$ does not depend on the direction, that is, it is isotropic. However, there are two types of $\alpha_c$ ($\alpha_{11}$ and $\alpha_{33}$) in langasite family crystals. In this study, $\alpha_{11}$ and $\alpha_{33}$ are defined as $\alpha_y (=\alpha_x)$ and $\alpha_z$, respectively. It is assumed that the external force applied from the crystal to the metal is equal to that applied from the metal to the crystal, and this is defined as the thermal stress $\sigma$. The thermal stress generated between the crystal and the metal was calculated at 400 °C, which was the maximum working temperature. Stainless steel, composed of iron and carbon, is normally used for the metal, and its LTEC $\alpha_m$ is assumed to be $11 \times 10^{-6} \text{ K}^{-1}$ in the calculation [19]. The $\alpha_y$ and $\alpha_z$ values of the langasite family crystals were determined in this study. As both the crystal and metal were fixed, as shown in Figure 1c, both the crystal and metal tend to expand to the same
length during heating. Therefore, the elongation λ of the crystal and metal from room temperature (23 °C) to the working temperature is expressed using the following Equations (3) and (4):

$$ \lambda = \Delta l_c + (\sigma / E_c) l_0, \qquad (3) $$

$$ \lambda = \Delta l_m + (-\sigma / E_m) l_0, \qquad (4) $$

where E_c is the elastic stiffness of the crystal and E_m is the Young’s modulus of the metal. In general, the LTEC of metals is larger than that of crystals. Therefore, the metal is stressed by the crystal in the negative direction, and the crystal is stressed in the opposite direction. Finally, the thermal stress σ can be calculated as:

$$ \sigma = \frac{(\alpha_m - \alpha_c)E_m E_c}{(E_m + E_c)} \Delta T, \qquad (5) $$

As mentioned above, anisotropic α_y and α_z should be considered, and we have treated two types of thermal stresses σ independent of each other. Therefore, σ_y and σ_z along the y and z directions of the crystal were calculated. In this study, the Young’s modulus of the metal was determined to be 152 GPa [19]. The elastic stiffness coefficients (EFC) of the crystal were determined by electroacoustic method, as described later. The aim of this study was to determine the ratio of σ_y and σ_z of the LTG crystal, σ_y/σ_z = 1 by element substitution.

<figure><img src="image_3.png" /><figcaption>**Figure 1.** Schematic of the thermal stress calculation process. (a) Initial state of the device element; (b) Thermal expansion of the crystal and metal; (c) Generated thermal stress.</figcaption></figure>

LTECs were obtained to investigate the thermal expansion anisotropy of order-type langasite family single crystals, as well as to calculate the thermal stress. The langasite-type crystals belong to the trigonal crystal system, point group 32, and space group P321. Thus, there are two independent expansion components, α₁₁ and α₃₃, along the crystallographic a- and c-axes, respectively. The LTECs were calculated using changes in the lattice constants a and c. Measurements were performed using a powder X-ray diffraction (XRD) method (Rigaku Ultim III SS), with a high-temperature furnace attachment, in the temperature range 23 to 500 °C, at intervals of 100 °C. We used Al₂O₃ polycrystal powder as the standard. The LTECs α₁₁ and α₃₃ were calculated by the following:

$$ \alpha_{11} = 1/a_0 \cdot \Delta a / \Delta T, \qquad (6) $$

$$ \alpha_{33} = 1/c_0 \cdot \Delta c / \Delta T, \qquad (7) $$

where a₀ (c₀), Δa (Δc), and ΔT represent the initial lattice constant of the sample at room temperature and the displacements and temperature change, respectively. The values of α₁₁ and α₃₃ correspond to α_y and α_z in Figure 1, respectively. As mentioned later, the LTG crystals show high anisotropic thermal stress, that is, high ratio of α_y and α_z.

In the crystal structure of the langasite family, there are four types of cation sites, and the chemical formula can be represented as A₃BC₃D₂O₁₄. The corresponding crystal structure is schematically shown in Figure 2. A and B represent the decahedral and octahedral sites, respectively; C and D represent tetrahedral sites, with the D site being smaller than the C site. In the LTG crystal, La³⁺ occupies the A sites, Ta⁵⁺ occupies half of the B sites, and Ga³⁺ occupies another half of the B sites and both the C and D sites. The langasite family crystals are classified into two types depending on their site occupation
patterns [20]. One is known as a disorder-type structure (such as LGS and LTG), in which at least one of the four cation sites is occupied by two or more different elements (Ta and Ga in LTG). The other is known as an order-type structure (such as $Sr_3TaGa_3Si_2O_{14}$), in which all cation sites are occupied by a single element [21]. In this study, we measured the LTEC using $Ca_3TaGa_3Si_2O_{14}$ (CTGS) [22], $Ba_3TaGa_3Si_2O_{14}$ (BTGS) [23], $Ca_3NbGa_3Si_2O_{14}$ (CNGS) [24], and $Ca_3TaAl_3Si_2O_{14}$ (CTAS) [25] crystals. By comparing the thermal stress ratio $\alpha_y/\alpha_z$ of each crystal, it was found that the four sites were effective in reducing the anisotropic thermal stress of the LTG crystal. The CTGS, BTGS, CNGS, and CTAS crystal ingots have been reported in other studies [22–25]. These crystals were pulverized and used for powder XRD. As mentioned later, we found that the largest cation A site affects the thermal stress. Then, we formulated an idea to replace $La^{3+}$ in LTG by larger ions, such as $Sr^{2+}$. On the basis of this idea, we attempted to grow strontium-substituted LTG (Sr-LTG) single crystals.

<figure><img src="image_4.png" /><figcaption>**Figure 2.** Schematic illustration of the langasite-type crystal structure viewed along the [001] direction.</figcaption></figure>

## 2.2. *Crystal Growth and Characterization*

Sr-LTG crystals were grown using a conventional RF-heating Czochralski (Cz) technique. Stoichiometric amounts of oxides and carbonates with 99.99% purity, corresponding to $La_{2.9}Sr_{0.1}Ta_{0.55}Ga_{5.45}O_{14}$ (Sr-LTG) were prepared and calcined at 1300 °C, for 5 h, in air. The chemical composition of the Sr-LTG was selected based on a previous study [26]. An iridium crucible was used with a diameter and height of 50 mm. The calcined powder was charged into a crucible. The growth atmosphere was achieved by flowing argon gas at $10^{-3} \text{ m}^3/\text{min}$ and oxygen gas at $10^{-5} \text{ m}^3/\text{min}$. A pure LTG single crystal bar was used as the seed. The pulling rate and rotation rates were 0.5 mm/h and 15 rpm, respectively. Phase identification of the as-grown crystals was performed by powder XRD. The crystal density was calculated using the lattice parameter, and the chemical composition was determined using an electron probe microanalyzer (EPMA).

In the Sr-LTG crystals, the independent material constants consisted of two dielectric, two piezoelectric, and six elastic compliance constants ($\varepsilon_{ij}$, $d_{ij}$, and $s_{ij}$, respectively). These material constants were determined using an impedance/gain phase analyzer (HP 4194A, Agilent) as reported previously [27,28]. The electromechanical coupling factor $k_{ij}$ and the piezoelectric modulus were evaluated by measuring the mechanical series resonance frequency $f_s$ and parallel resonance frequency $f_p$ of the equivalent resonators. The equivalent resonators were fabricated in the form of plates according to the length-extensional vibration mode. The dielectric constants, $\varepsilon_{ij}$, were determined by measuring the capacitances of the resonators by considering the parasitic capacitance.

# 3. *Results and Discussion*

Figure 3 shows the temperature dependence of the lattice constants along the crystallographic *a*- and *c*-axes of the $Ba_3TaGa_3Si_2O_{14}$ (BTGS) crystal. These lattice constants changed linearly across the entire temperature range. The calculated LTEC of the *a*-axis was almost the same as that of the *c*-axis, as shown in Table 1. The LTECs at 400 °C were all positive, indicating that the LTEC of the BTGS crystal is anisotropic. To calculate the thermal stress for the langasite family crystals, the LTECs of $Ca_3TaGa_3Si_2O_{14}$, $Ca_3NbGa_3Si_2O_{14}$, $Ca_3TaAl_3Si_2O_{14}$, and $La_3Ta_{0.5}Ga_{5.5}O_{14}$ crystals were also measured
using the same process used for the BTGS crystal. All the LTECs and the elastic stiffness data are provided in Table 1 for the calculation of the thermal stresses.

<figure><img src="image_5.png" /><figcaption>**Figure 3.** Dependence of the lattice constants on the temperature of the Ba₃TaGa₃Si₂O₁₄ crystal along the crystallographic (a) *a*-axis and (b) *c*-axis. Linear thermal expansion coefficients are also shown inside.</figcaption></figure>

<table><caption>**Table 1.** Elastic stiffness coefficients (ESCs) and linear thermal expansion coefficients (LTECs) of the langasite family crystals. CTGS, BTGS, CNGS, CTAS, and LTG are the abbreviations for Ca₃TaGa₃Si₂O₁₄ [22], Ba₃TaGa₃Si₂O₁₄ [23], Ca₃NbGa₃Si₂O₁₄ [24], Ca₃TaAl₃Si₂O₁₄ [25], La₃Ta₀.₅Ga₅.₅O₁₄ [29], respectively.</caption><thead><tr><th rowspan="2">Crystal</th><th colspan="2">ESC (GPa)</th><th colspan="2">TEC (10<sup>-6</sup> K<sup>-1</sup>)</th></tr><tr><th>c<sub>y</sub></th><th>c<sub>z</sub></th><th>α<sub>y</sub></th><th>α<sub>z</sub></th></tr></thead><tbody><tr><td>CTGS</td><td>123.2</td><td>178.1</td><td>8.30</td><td>7.13</td></tr><tr><td>BTGS</td><td>211.0</td><td>423.0</td><td>5.52</td><td>8.02</td></tr><tr><td>CNGS</td><td>155.0</td><td>226.0</td><td>8.02</td><td>7.70</td></tr><tr><td>CTAS</td><td>184.4</td><td>477.4</td><td>8.08</td><td>8.12</td></tr><tr><td>LTG</td><td>189.8</td><td>263.5</td><td>7.99</td><td>5.97</td></tr></tbody></table>

ESC were calculated using the data reported in [22–25,29].

Using the ESCs and LTECs in Table 1, the thermal stresses were calculated using Equation (5) and are presented in Figure 4. The thermal stress of the LTG crystal, the most promising candidate for the combustion pressure sensor, was also calculated. The data of the LTG crystal were calculated using the values reported in previous studies [29,30]. As $\sigma_y$ was twice the $\sigma_z$ value in the LTG crystal, the anisotropy of thermal stress was high. There are two possible methods to reduce the anisotropy of thermal stress in LTG crystals. One method is to increase $\sigma_y$, and the other method is to decrease $\sigma_z$. By comparing the $\sigma_y$ of CTGS, BTGS, CNGS, and CTAS crystals, it was demonstrated that the A site ion with a higher ionic radius effectively increased the value of $\sigma_y$. However, as the $\sigma_z$ values were the same in all the crystals used in this study, it was inferred that not all substituent elements led to a decrease in the $\sigma_z$ of the LTG. Therefore, by substituting atoms with larger ionic radii for the A site, such as CTGS and BTGS, it was expected that the anisotropy of the thermal stress could be reduced by increasing $\sigma_y$. Bi³⁺ (1.17 Å), Na⁺ (1.18 Å), Sr²⁺ (1.26 Å), Pb²⁺ (1.29 Å), and Ba²⁺ (1.42 Å) were possible candidates for ions with an ionic radius larger than that of La³⁺ (1.16 Å) [31]. The ionic radii of Bi³⁺ and Na⁺ are almost the same as that of La, and the change in the anisotropy of the thermal stress should be small. Moreover, Pb²⁺ was excluded because of its toxicity, and Ba²⁺ was not considered because it is difficult to introduce Ba²⁺ into the LTG crystal lattice [26]. Therefore, in the present study, the growth of Sr-LTG single crystals was attempted based on a previous study [26].
<figure><img src="image_6.png" /><figcaption>**Figure 4.** Thermal stress, $\sigma_y$ and $\sigma_z$, of the langasite family crystals at 400 °C along the [120] (y-axis) and c-axis, respectively. The data were calculated using the elastic stiffness coefficients (ESCs), linear thermal expansion coefficients (LTECs) shown in Table 1. CTGS, BTGS, CNGS, CTAS, and LTG are the abbreviations for Ca₃TaGa₃Si₂O₁₄, Ba₃TaGa₃Si₂O₁₄, Ca₃NbGa₃Si₂O₁₄, Ca₃TaAl₃Si₂O₁₄, La₃Ta₀.₅Ga₅.₅O₁₄, respectively.</figcaption></figure>

Growth of Sr-LTG crystals has been reported [26], and therefore the starting composition of Sr-LTG was set as La₂.₉Sr₀.₁Ta₀.₅₅Ga₅.₄₅O₁₄. The Sr-LTG single crystal without any inclusions was successfully grown by the Cz method, as shown in Figure 5. The Sr-LTG crystals grown, in this study, were transparent, orange in color, and 23 mm in diameter and 70 mm in length. The upper part of the boule contained six developed flat surfaces, which consisted of planes parallel to the <001> growth direction. Backscattering Laue X-ray analysis showed that the flat surfaces correspond to {100} planes. Small cracks and bubbles were observed in the lower part of the boule. All peaks of the crystal powder XRD patterns agreed with those of the LTG structure. We carefully eliminated these macro defects via proper sample preparation, including cutting and polishing, for material constant measurement. The solidification fraction, $g = W_{crystal}/W_{initial}$, where $W_{crystal}$ and $W_{initial}$ are the weights of the grown crystal and the starting melt, respectively, was 0.36. The Sr content of the LTG crystal was smaller than that of the starting raw materials, taking into account the accuracy of EPMA analysis conducted in this study. This result agrees well with that reported in [26]. The grown crystal was pulverized, and its powder was also used for measurement of LTEC.

<figure><img src="image_7.png" /><figcaption>**Figure 5.** Photograph of side view of strontium-substituted LTG (Sr-LTG) crystals grown by the Czochralski (Cz) method.</figcaption></figure>

The ESC and LTEC of the Sr-LTG crystal were measured, and the thermal stresses $\sigma_y$ and $\sigma_z$ were calculated and are listed in Table 2, along with those of the LTG crystal [29]. The ESCs, $c_y$ and $c_z$, were higher and lower, respectively, for Sr-LTG than for LTG, indicating that the LTG crystal lattice was hardened along the direction perpendicular to the c-axis and softened along the c-axis, due to Sr substitution, respectively. The reasons for this should be clarified from the viewpoint of changes to crystal structure by Sr substitution. Detailed structural analysis is currently under investigation.
The thermal stresses, $\alpha_y$ and $\alpha_z$, of the Sr-LTG crystal were higher and lower than those of the LTG crystal, respectively. Thus, the thermal stress ratio $\alpha_y/\alpha_z$ of the Sr-LTG crystal was closer to unity than that of the LTG crystal. Consequently, the anisotropy of the thermal stress was effectively reduced by the Sr substitution into the LTG lattice. Electromechanical properties were characterized using the $(XYt)\theta^\circ(\theta = 0, 30, 60, \text{ and } -30)$ substrates of the Sr-LTG crystals. The $d_{11}$ values determined were 5.81 pC/N for the Sr-LTG. The magnitude of the piezoelectric $d_{11}$ coefficient for Sr-LTG was lower than that for LTG (7.06 pC/N [32]). The reduction by Sr substitution has been previously reported [26]. The reason for this remains under consideration and will be clarified by combining the detailed crystal structural analysis and characterization of all the electromechanical coefficients. The $d_{11}$ coefficient was still higher than the $d_{11}$ values of quartz (2.30 pC/N [33]), and hence suggested that the Sr-LTG crystal is a superior candidate material for combustion pressure sensors.

<table><caption>**Table 2.** Elastic stiffness coefficients (ESCs), linear thermal expansion coefficients (LTECs), thermal stresses, and the ratio of LTG and Sr-LTG crystals.</caption><thead><tr><th rowspan="2">Crystal</th><th colspan="2">ESC (GPa)</th><th colspan="2">LTEC (10<sup>-6</sup> K<sup>-1</sup>)</th><th colspan="2">Thermal Stress (MPa)</th><th rowspan="2">Ratio</th></tr><tr><th>c<sub>y</sub></th><th>c<sub>z</sub></th><th>α<sub>y</sub></th><th>α<sub>z</sub></th><th>σ<sub>y</sub></th><th>σ<sub>z</sub></th></tr></thead><tbody><tr><td>LTG [29,30]</td><td>189.8</td><td>263.5</td><td>7.99</td><td>5.97</td><td>101.9</td><td>193.9</td><td>0.53</td></tr><tr><td>Sr-LTG</td><td>206</td><td>214</td><td>7.80</td><td>6.43</td><td>112.2</td><td>162.5</td><td>0.69</td></tr></tbody></table>

## 4. Conclusions

In this study, we formulated a method to reduce the anisotropy of the thermal stress generated on LTG crystals when the LTG crystal was used as a combustion pressure sensor. This was achieved by comparing the anisotropy of the thermal stress of order-type langasite family crystals. The solution included the A site (La<sup>3+</sup>) in the LTG crystal being substituted with the larger Sr<sup>2+</sup> ions. Therefore, the crystal growth of Sr-LTG was undertaken using the Cz method. The Sr-LTG single crystal without any inclusions was successfully grown. By Sr substitution, the thermal stress ratio $\alpha_y/\alpha_z$ of the LTG crystal was effectively reduced, while maintaining the piezoelectric property. We conclude that the Sr-LTG single crystal is a superior candidate material for pressure sensors usable at high temperatures.

**Author Contributions:** Conceptualization, H.T. and H.U.; methodology, H.T., H.U., M.T., K.S. and K.L.; software, T.H. and T.T.; writing—original draft preparation, H.T.; writing—review and editing, T.H., T.T. and I.Y.; funding acquisition, H.T. All authors have read and agreed to the published version of the manuscript.

**Funding:** This research was funded by JSPS KAKENHI, grant number 19H02797.

**Acknowledgments:** We would like to thank Kiyoshi Shimamura of NIMS, Japan, and Tomoaki Karaki of Toyama Pref. University, Japan and Katsumi Kawasaki of TDK Corp., Japan for providing crystal samples with CTGS (K.S.), CTAS (K.S.), CNGS (T.K.) and BTGS (K.K.), respectively. We are also grateful to Masaru Tada, Tokyo Institute of Technology, Japan for the technical support in the EPMA analysis.

**Conflicts of Interest:** The authors declare no conflict of interest.

## References

1. Rogers, D.R. *Engine Combustion: Pressure Measurement and Analysis*; SAE International: Warrendale, PA, USA, 2010.

2. Tsukada, K.; Takeuchi, M.; Tokumitsu, S.; Ohmura, Y.; Kawaguchi, K. Combustion pressure sensor. *R&D Rev. Toyota CRDL* **1993**, *28*, 49–57. (In Japanese)

3. Shimamura, K.; Takeda, H.; Kohno, T.; Fukuda, T. Growth and characterization of lanthanum gallium silicate La<sub>3</sub>Ga<sub>5</sub>SiO<sub>14</sub> single crystals for piezoelectric application. *J. Cryst. Growth* **1996**, *163*, 388–392. [CrossRef]

4. Takeda, H.; Shimamura, K.; Kohno, T.; Fukuda, T. Growth and Characterization of La<sub>3</sub>Nb<sub>0.5</sub>Ga<sub>5.5</sub>O<sub>14</sub> Single Crystals. *J. Cryst. Growth* **1996**, *169*, 503–508. [CrossRef]

5. Bohm, J.; Heimann, R.B.; Hengst, M.; Roewer, R.; Schindler, J. Czochralski growth and characterization of piezoelectric single crystals with langasite structure: La<sub>3</sub>Ga<sub>5</sub>SiO<sub>14</sub> (LGS), La<sub>3</sub>Ga<sub>5.5</sub>Nb<sub>0.5</sub>O<sub>14</sub> (LGN), and La<sub>3</sub>Ga<sub>5.5</sub>Ta<sub>0.5</sub>O<sub>14</sub> (LGT). Part I. *J. Cryst. Growth* **1999**, *204*, 128–136. [CrossRef]
6. Takeda, H.; Fukuda, T.; Kawanaka, H.; Onozato, N. Effect of starting melt composition on growth of La₃Ta₀.₅Ga₅.₅O₁₄ crystal. *J. Mater. Sci. Mater. Electron.* **2001**, *12*, 199–202. [CrossRef]

7. Uda, S.; Wang, S.Q.; Konishi, N.; Inaba, H.; Harada, J. Growth habits of 3 and 4-inch langasite single crystals. *J. Cryst. Growth* **2002**, *237*, 707–713. [CrossRef]

8. Boutahraoui, B.; Nehari, A.; Boy, J.J.; Vacheret, X.; Allani, M.; Cabane, H.; Dumortier, M.; Derbal, M.; Lebbou, K. LGT (La₃Ga₅.₅Ta₀.₅O₁₄) langatate bulk crystal grown from the melt by Czochralski technique and characterization. *Opt. Mater.* **2017**, *65*, 103–105. [CrossRef]

9. Allani, M.; Batis, N.; Laroche, T.; Nehari, A.; Cabane, H.; Lebbou, K.; Vacheret, X.; Boy, J.J. Effects of the Langatate crystal quality on the resonance frequency stability of bulk acoustic wave resonators. *Adv. Appl. Ceram.* **2018**, *117*, 279–284. [CrossRef]

10. Krempl, P.; Schleinzer, G.; Wallnöfer, W. Gallium phosphate, GaPO₄: A new piezoelectric crystal material for high-temperature sensorics. *Sens. Actuators A Phys.* **1997**, *61*, 361–363. [CrossRef]

11. Yu, F.; Zhang, S.; Zhao, X.; Yuan, D.; Qin, L.; Wang, Q.-M.; Shrout, T.R. Dielectric and electromechanical properties of rare earth calcium oxyborate piezoelectric crystals at high temperatures. *IEEE Trans. Ultra. Ferro. Freq. Contr.* **2011**, *58*, 868–873.

12. Balitsky, D.V.; Philippot, E.; Papet, P.; Balitsky, V.S.; Pey, F. Comparative crystal growth of GaPO₄ crystals in the retrograde and direct solubility range by hydrothermal methods of temperature gradient. *J. Cryst. Growth* **2005**, *275*, e887–e894. [CrossRef]

13. Takeda, H.; Sako, H.; Shimizu, H.; Kodama, K.; Nishida, M.; Nakao, H.; Nishida, T.; Okamura, S.; Shikida, T.; Shiosaki, T. Growth and characterization of lanthanum Calcium Oxoborate LaCa₄O(BO₃)₃ single crystals. *Jpn. J. Appl. Phys.* **2003**, *42*, 6081–6085. [CrossRef]

14. Takeda, H.; Hagiwara, M.; Noguchi, H.; Hoshina, T.; Takahashi, T.; Kodama, N.; Tsurumi, T. Calcium aluminate silicate Ca₂Al₂SiO₇ single crystal applicable to piezoelectric sensors at high temperature. *Appl. Phys. Lett.* **2013**, *102*, 242907. [CrossRef]

15. Shen, C.; Zhang, S.; Cao, W.; Cong, H.; Yu, H.; Wang, J.; Zhang, H. Thermal and electromechanical properties of melilite-type piezoelectric single crystals. *J. Appl. Phys.* **2015**, *117*, 064106. [CrossRef]

16. Yaokawa, R.; Kimura, H.; Aota, K.; Uda, S. Precipitation phenomena in and electrical resistivity of high-temperature treated langatate (La₃Ta₀.₅Ga₅.₅O₁₄). *IEEE Trans. Ultra. Ferro. Freq. Contr.* **2011**, *58*, 1131–1139. [CrossRef] [PubMed]

17. Spassky, D.A.; Kozlova, N.S.; Kozlova, A.P.; Zabelina, E.V.; Buzanov, O.A.; Buryi, M.; Laguta, V.; Lebbou, K.; Nehari, A.; Cabane, H.; et al. Study of the defects in La₃Ta₀.₅Ga₅.₅O₁₄ single crystals. *J. Lumin.* **2016**, *180*, 95–102. [CrossRef]

18. Takahashi, I.; CITIZEN FINEDEVICE CO., LTD, Fujikawaguchiko-Machi, Yamanashi, Japan. Personal communication, 2019.

19. Kasano, H.; Hara, T.; Minakuchi, Y. Thermal stress (Netsuouryoku). In *Fundamental of Mechanics of Materials (Kisozairyorikigaku)*, 1st ed.; Koizumi, T., Ed.; Yokendo: Tokyo, Japan, 2014; pp. 30–33. (In Japanese)

20. Wang, Z.; Cheng, X.; Yuan, D.; Pan, L.; Guo, S.; Xu, D.; Lv, M. Crystal growth and properties of Ca₃NbGa₃Si₂O₁₄ single crystals. *J. Cryst. Growth* **2003**, *249*, 240–244. [CrossRef]

21. Takeda, H.; Sato, J.; Kato, T.; Kawasaki, K.; Morikoshi, H.; Shimamura, K.; Fukuda, T. Synthesis and characterization of Sr₃TaGa₃Si₂O₁₄ single crystals. *Mater. Res. Bull.* **2000**, *35*, 245–252. [CrossRef]

22. Shi, X.; Yuan, D.; Yin, X.; Wei, A.; Guo, S.; Yu, F. Crystal growth and dielectric, piezoelectric and elastic properties of Ca₃TaGa₃Si₂O₁₄ single crystal. *Solid State Commun.* **2007**, *142*, 173–176. [CrossRef]

23. Usui, H.; Kusakabe, H.; Tokuda, M.; Sugiyama, K.; Hoshina, T.; Tsurumi, T.; Takeda, H. Structure and electrical properties of Ba₃TaGa₃Si₂O₁₄ single crystals grown by Czochralski method. *J. Ceram. Soc. Jpn.* **2020**, *128*, 441–446. [CrossRef]

24. Karaki, T.; Sato, R.; Adachi, M.; Kushibiki, J.; Arakawa, M. Piezoelectric properties of Ca₃NbGa₃Si₂O₁₄ single crystal. *Jpn. J. Appl. Phys.* **2004**, *43*, 6721–6724. [CrossRef]

25. Fu, X.; Víllora, E.G.; Matsushita, Y.; Kitanaka, Y.; Noguchi, Y.; Miyayama, M.; Shimamura, K.; Ohashi, N. Piezoelectric Ca₃TaAl₃Si₂O₁₄ (CTAS): High quality 2-in. single-crystal growth and electro-elastic properties from room to high (650 °C) temperature. *J. Cryst. Growth* **2018**, *501*, 38–42. [CrossRef]

26. Takeda, H.; Kato, T.; Chani, V.I.; Morikoshi, H.; Shimamura, K.; Fukuda, T. Effect of (Sr, Ba) substitution in La₃Ga₅SiO₁₄ and La₃M₀.₅Ga₅.₅O₁₄ (M = Nb⁵⁺, Ta⁵⁺) crystals on their synthesis, structure and piezoelectricity. *J. Alloys Compd.* **1999**, *290*, 79–84. [CrossRef]
27. ANSI/IEEE Std 176. *IEEE Standard on Piezoelectricity*; IEEE: New York, NY, USA, 1987.

28. Ikeda, T. *Fundamentals of Piezoelectricity*; Oxford University Press: New York, NY, USA, 1990.

29. Chilla, E.; Flannery, C.M.; Frohlich, H.-J.; Straube, U. Elastic properties of langasite-type crystals determined by bulk and surface acoustic waves. *J. Appl. Phys.* **2001**, *90*, 6084–6091. [CrossRef]

30. Beaucage, T.R.; Beenfeldt, E.P.; Speakman, S.A.; Porter, W.D.; Payzant, E.A.; Pereira Da Cunha, M. Comparison of high temperature crystal lattice and bulk thermal expansion measurements of LGT single crystal. In Proceedings of the 2006 IEEE International Frequency Control Symposium and Exposition, Miami, FL, USA, 4–7 June 2006; pp. 658–663.

31. Shannon, R.D. Revised effective ionic radii and systematic studies of interatomic distances in halides and chalcogenides. *Acta Crystallogr. A* **1976**, *32*, 751–766. [CrossRef]

32. Bohm, J.; Chilla, E.; Flannery, C.; Frohlich, H.-J.; Hauke, T.; Heimann, R.B.; Hengst, M.; Straube, U. Czochralski growth and characterization of piezoelectric single crystals with langasite structure: La₃Ga₅SiO₁₄ (LGS), La₃Ga₅.₅Nb₀.₅O₁₄ (LGN) and La₃Ga₅.₅Ta₀.₅O₁₄ (LGT) II. Piezoelectric and elastic properties. *J. Cryst. Growth* **2000**, *216*, 293–298. [CrossRef]

33. Trolier-McKinstry, S.; Cross, L.E.; Yamashita, Y. (Eds.) *Piezoelectric Single Crystals and Their Applications*; Pennsylvania State University: University Park, PA, USA, 2004.

**Publisher's Note:** MDPI stays neutral with regard to jurisdictional claims in published maps and institutional affiliations.

<figure><img src="image_8.png" /></figure>

© 2020 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).